| ||Format||Pages||Price|| |
|3||$41.00||  ADD TO CART|
|Hardcopy (shipping and handling)||3||$41.00||  ADD TO CART|
Significance and Use
3.1 The modulus of rupture of carbon-containing refractories at elevated temperatures has become accepted as a useful measurement in quality control testing and in research and development. These measurements are also used to determine the suitability of particular products for various applications and to develop specifications. The sample may undergo some oxidation during the test.
3.3 Resin bonded magnesia-carbon brick containing approximately 17 % carbon after coking where tested in two separate ruggedness tests. Metal-free brick were tested in the first ruggedness test, while aluminum-containing brick were tested in the second. Results were analyzed at a 95 % confidence level.
3.4 For the metal-free brick, the presence of an argon atmosphere and hold time had statistically significant effects on the modulus of rupture at 2550°F (1400°C). The argon atmosphere yielded a lower modulus of rupture. The samples tested in air had a well-sintered decarburized zone on the exterior surfaces, possibly explaining the higher moduli of rupture. The longer hold time caused a lower result for the metal-free brick.
3.5 For the aluminum-containing brick, testing temperature, the presence of an argon atmosphere, and loading rate had statistically significant effects on the modulus of rupture at 2550°F (1400°C). The higher testing temperature increased the measured result, the presence of an argon atmosphere lowered the result, and the higher loading rate increased the result.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. For specific hazard statements, see Section 5.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C583 Test Method for Modulus of Rupture of Refractory Materials at Elevated Temperatures
E220 Test Method for Calibration of Thermocouples By Comparison Techniques
ISO StandardISO Recommendation 5013 Determination of the Hot Modulus of Rupture of Shaped and Unshaped Dense and Insulating Refractory Products Available from American National Standards Institute (ANSI), 25 W. 43rd St., 4th Floor, New York, NY 10036, http://www.ansi.org.
ICS Number Code 81.080 (Refractories)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM C1099-07(2012), Standard Test Method for Modulus of Rupture of Carbon-Containing Refractory Materials at Elevated Temperatures, ASTM International, West Conshohocken, PA, 2012, www.astm.orgBack to Top